- Nano Express
- Open Access
Design parameters for enhanced photon absorption in vertically aligned silicon nanowire arrays
Nanoscale Research Lettersvolume 9, Article number: 511 (2014)
Superior photon absorption in ordered nanowire arrays has been demonstrated recently. However, systematic studies are still missing to explore the limits of their implementation as functional photonic devices. With emphasis on silicon nanowires, we investigated the effects of nanowire diameter, length, morphology, and pitch on the photon absorption within the visible solar spectrum based on simulations. Our results reveal that these parameters are crucial but disclose a path to improve the absorbance drastically.
78.40.Fy; 78.67.Uh; 78.67.-n
Photon harvesting is one key factor determining the performance of photonic devices such as solar cells and photodetectors. In recent years, promising improvements could be accomplished for photon management utilizing nanostructures such as wires, cones, dots, pyramids, and cubes to lower the reflectivity , increase the absorption over broad wavelength ranges , and to reduce the dependency on the angle of light incidence [2–4]. Despite these achievements, further systematic studies are required to enable rational tailoring of nanoscale morphologies with respect to the optical application. Within the range of potential nanostructures, nanowires (NW) are one important class [5–9]. The focus of this work is put on silicon nanowires (SiNWs), which have been in discussion for a while as effective structures to drastically improve the photon absorption probability especially if aligned in parallel to the angle of light incidence [10, 11]. Aside from this passive exploitation of the geometry, SiNWs can possess a p-n junction as well allowing their direct use for solar energy conversion if assembled as photonic device [12–17]. In terms of the material, silicon is still leading for semiconductor photovoltaic applications but is also vastly used in various microfabricated electronic devices enabling perfect alignment of silicon nanostructures with common standards in technology. Aligned SiNW arrays can be fabricated bottom-up, e.g., by the vapor-liquid-solid method (VLS, Figure 1a)  or by top-down etching techniques . Although both methods have their intrinsic advantages and disadvantages, they have in common that with respect to the geometry, the average nanowire pitch, length, diameter, and overall morphology such as nanowire tapering can in principle be rationally adjusted. As shown in individual experiments, these parameters are key factors for the resulting optical properties [20, 21]. For instance, Zhu et al. showed that tapered SiNWs excel over cylindrical nanowires in terms of a minimized reflectivity . To explore the limits of silicon nanowire arrays utilized for photonic applications, we performed comprehensive three-dimensional (3D) simulations for idealized vertical SiNW arrays in comparison to the literature and mainly thin single crystalline silicon membranes. From the simulations, a general set of design parameters can be deduced, enabling to pre-evaluate the optical properties depending on the geometrical conditions preventing intrinsic design-based deficiencies of devices within experiments.
The 3D optical simulations were realized by means of the finite element method (FEM). FEM simulations are very suitable to simulate NW arrays with various shapes as they use a variable mesh to model the desired geometry. In principle, two NW shapes were studied: NWs with a constant diameter D (cylindrical NWs, Figure 1b,c) and tapered NWs with a linear transition from a fixed bottom diameter to a smaller top diameter (Figure 1d). To describe wavelength-dependent light-matter interaction, all simulations were conducted in the frequency domain and were based on Maxwell’s equations but without considering thermal effects. Although the infrared wavelength regime is important, the following studies focus on the spectral range from 300 to 800 nm. This is based on the fact that SiNW arrays and thin Si membranes do not show any significant absorption above 800 nm in contrary to bulk silicon [see Additional file 1: Figure S1] . For all considered scenarios, the simulated sample comprised of a homogenous infinite set of nanowires placed in air with a specific NW length and periodic pitch (Figure 1b). The infinite NW array eliminates the influence of any boundary effects and is created by periodic repetition of a single nanowire element in two lateral directions. Consequently, all results can be ascribed to geometric and material effects solely. Material parameters were implemented in our simulations as wavelength-dependent complex refractive indices [see Additional file 1: Figure S1]. The optical illumination spectrum was realized with electromagnetic waves propagating as plane waves perpendicular to the surface and parallel to the NWs longitudinal axis and was, if not stated otherwise, weighted with an air-mass 1.5 global (AM 1.5G) solar spectrum . The optical transmittance and reflectance were directly extracted from the simulations depending on the wavelength in the aforementioned range of 300 to 800 nm with an increment of 10 nm. For comparison purposes, the ideal short circuit current density JSC was calclulated from the obtained absorption spectrum considering an internal quantum efficiency of 0.8 (approximately mean value from ) and 1 sun illumination. With respect to maximum accuracy, the FEM mesh size was chosen to be much smaller than the simulated wavelengths with a varying edge length between 14 and 30 nm. Finally, the absorbance was determined from the simple relation that the summation of transmittance, reflectance, and absorbance equals one. All simulations were conducted under similar conditions. Therefore, the calculated short circuit current density leads to a numeric value suitable to quantitatively compare the presented simulations among each other and even with experiments (Figure 2a). Our simulations were performed without a substrate in order to keep the obtained results as generic as possible with emphasis on nanowires and unaffected from a substrate material (e.g., additional reflection or absorption). Hence, the nanowire array is basically floating in air enabling us to evaluate its optical behavior solely. This approach is supported by van de Groep and Polman , who showed that a substrate material is mainly influencing the absolute values while the overall characteristics and trends are governed by the used nanostructures.
Results and discussion
To validate our simulation approach experimentally, a single crystalline (100) silicon wafer was spectroscopically characterized, allowing us to extract the absorbance depending on the wavelength. In Figure 2a, these values are compared to the results deduced from our simulation considering a planar structure with infinite thickness. The results show that our simulation can appropriately predict the optical behavior of a real bulk silicon sample. Optical characterizations performed by other groups with SiNW arrays are also qualitatively in suitable agreement with our results . However, a quantitative comparison would require samples with well-defined structures over large scales and the full experimental parameter set if published elsewhere. While until now, these constraints appear unfulfilled for SiNW arrays; results published by Fan et al.  for germanium (Ge) NW arrays appear adequate. In this paper, cylindrical NWs with 2 µm in length and 80 nm in diameter, both average values, are arranged with an average pitch of 150 nm on a glass substrate. Taking the ideal character of the simulations, the tabulated optical properties, and the experimental conditions into account, the simulation is in convincing agreement (Figure 2a).
A first pre-evaluation of a substrate-free SiNW array, equal to the aforementioned GeNW array, is shown in comparison to a planar Si membrane in Figure 2b. To enable a comparison, the membrane thickness and the NW length were both fixed to 2 µm. These simulations indicate that the SiNW array exhibits a significantly increased absorption (approximately factor 1.4) over a large spectral range. This is even more supported by the fact that in this case, the NW array volume is less then 23% of the membrane material volume. A straightforward explanation is the higher bulk surface reflectivity. In the visible wavelength range, a mean ratio of about 50% of incident light is reflected in case of silicon and is therefore not coupled into the material. In contrast, NW arrays and the surrounding air are minimizing reflective losses by creating an effective refractive index. Its value or gradient depends intrinsically on the NW geometry and arrangement which is also pointed out, e.g., by Patchett et al. , which even enables us to rationally customize spectral absorption characteristics [see Additional file 1: Figure S2]. However, the focus of this study is to maximize the absorption or short circuit current density in NW arrays depending on the parameters NW diameter, morphology, length, and pitch. If the spectral characteristics of the silicon examples given in Figure 2a,b are compared to previous works, it can be deduced that the longer wavelength regime is suppressed as a result of the distinct material volume and thickness (NW length) dependency of the optical absorption .
To evaluate material volume effects, the NW diameter and length were varied from 50 to 200 nm and from 0.5 to 2 µm, respectively, using a constant pitch of 250 nm (Figure 3). Figure 3 shows that the short circuit current density increases with increasing length and diameter (total absorption is provided in Additional file 1: Figure S5 to S8). However, the gain in current density is not proportional to the gain in material volume. For instance, only moderate current density improvements can be achieved for diameters larger than 100 nm, which stands in striking contrast to the strong increase for smaller diameters. Depending on the diameter, but also pitch, the silicon/air volume ratio varies strongly. For instance, a diameter of 150 nm and a pitch of 250 nm make up for a volume filling of silicon of about 30%. However, a short circuit current density enhancement of about 70% is achieved. Here, mainly two effects contribute to these results. The effect of the diameter can be simply understood by considering the aforementioned effective refractive index approximation . On the one hand, the material volume and therefore, the short circuit current density, is increased with increasing diameter. On the other hand, the reflection coefficient is increased as well based on the fact that the structure is continuously approaching its bulk state . In case of the length, the absorption is dominated by the upper part of the NW (Figure 3 inset). Therefore, the gain in absorption and short circuit current density declines non-linearly with increasing length. From the simulations, a representable absorption coefficient based on 100 nm NW diameter and 250 nm pitch for 500 nm wavelength of 1.3×106 1/m could be extracted. This means that 90% of the incident light is already absorbed within the first 1.8 µm in this case.The pitch, which was kept constant at 250 nm before, should now be evaluated exemplary for a NW length of 1 µm and a diameter of 100 nm within a range of 125 to 500 nm referring to the highest and lowest NW density, respectively. As shown in Figure 4, the short circuit current density has a maximum in the range of 150 to 200 nm pitch and decreases to both sides. Above 200 nm, the current density declines almost linearly until it approaches the short circuit current density for planar membrane silicon.
Based on the discussed fact that the absolute value of the short circuit current density depends strongly on the pitch and diameter, both must also be evaluated simultaneously in order to determine the global maximum in photon absorption or current density, as shown in Figure 5. This maximum is shifted towards the micron scale and can be found at a pitch of 500 nm using cylindrical wires of 350 nm in diameter. For these parameters, the maximum short circuit current density is obtained with a value of 13.9 mA/cm 2, which is over a factor of two higher than 5.8 mA/cm 2 obtained for a silicon membrane of 1 µm in thickness. In general, a characteristic local maximum can be expected if the D/P ratio is in the range of 0.7 to 0.8, which is in alignment with estimates published elsewhere [27–29].
Until now, only SiNWs with cylindrical geometry were considered in the discussion. However, in reality, the axial geometry can easily differ from this model being more conical or frustum like (Figure 1d). Such tapered structures are, for instance, readily obtained for VLS synthesis if a lateral overgrowth is present besides the axial NW elongation. In principle, tapered NW structures possess an axial linear diameter gradient providing simultaneously an axial gradient for the effective refractive index. However, a thorough discussion of tapering effects is complex and depends strongly on the aspired application. To be in alignment with the previous simulations, NWs with 100 nm in diameter are considered exemplarily as depicted in Figure 6. Therefore, NW arrays were studied with a fixed NW bottom diameter of 100 nm while the top diameter was varied from 0 nm (ideal sharp tip) to 100 nm (cylindrical NW). Any structure in between is consequently a truncated cone. As shown in Figure 6, strong tapering with a top diameter of less then 60 nm does not provide a benefit in terms of a maximized photon absorption or short circuit current density. Nevertheless, moderate tapering or truncated cones can represent an ideal geometry (see 350 nm pitch in Figure 6). This is as well valid for the previously derived global maximum with 350 nm NW diameter at 500 nm pitch. If this structure is turned into a truncated cone with 250 nm top diameter, the short circuit current density can be further increased by 9.4% to 15.2 mA/cm 2. In general, the achievable enhancement or the ideal geometry depends strongly on all geometric factors like diameter, length, and pitch influencing again the tradeoff between volume and effective index of refraction.
A NW shape tending towards a cylinder should in general perform better than highly tapered nanowires. This is also still in agreement with the reported low reflectance values for strongly tapered nanowires situated on a substrate [1, 30]. Tapered NW arrangements benefit from an enhanced anti-reflection effect based on the tunable gradient of the effective refractive index from air to bulk material. This allows to maximize the transmittance or to minimize substrate reflectance if required for the application [see Additional file 1: Figure S3 and Additional file 1: Figure S4].
In conclusion, we evaluated the absorption characteristics of ordered arrays of vertically aligned silicon nanowires depending on their diameter, pitch, length, and shape using comprehensive 3D FEM simulations. From the simulations, the short circuit current density was derived, and we showed that silicon NW arrays can surpass the absorbance of silicon membranes. The global maximum of the short circuit current density for cylindrically shaped NWs could be predicted for approx. 350 nm diameter with 500 nm pitch with a short circuit current density of 13.9 mA/cm 2. This value can be further increased to 15.2 mA/cm 2 if the NWs represent a truncated cone with 250 nm top diameter. However, the implementation of highly tapered nanowires cannot be recommended in general if a maximum short circuit current density should be achieved within the NW array at minimum material volume.
finite element method
- J SC:
short circuit current density
Jung J-Y, Guo Z, Jee S-W, Um H-D, Park K-T, Lee J-H: A strong antireflective solar cell prepared by tapering silicon nanowires. Opt Express 2010, 18(S3):286–292. 10.1364/OE.18.00A286
Spinelli P, Verschuuren MA, Polman A: Broadband omnidirectional antireflection coating based on subwavelength surface mie resonators. Nat Commun 2012, 3: 692–16925.
Cao L, Fan P, Vasudev AP, White JS, Yu Z, Cai W, Schuller JA, Fan S, Brongersma ML: Semiconductor nanowire optical antenna solar absorbers. Nano Lett 2010, 10(2):439–445. 10.1021/nl9036627
Demesy G, John S: Solar energy trapping with modulated silicon nanowire photonic crystals. J Appl Phys 2012, 112(7):074326. 10.1063/1.4752775
Chen C, Jia R, Yue H, Li H, Liu X, Wu D, Ding W, Ye T, Kasai S, Tamotsu H, Chu J, Wang S: Silicon nanowire-array-textured solar cells for photovoltaic application. J Appl Phys 2010, 108(9):094318. 10.1063/1.3493733
Diedenhofen SL, Janssen OTA, Grzela G, Bakkers EPAM, Gómez Rivas J: Strong geometrical dependence of the absorption of light in arrays of semiconductor nanowires. ACS Nano 2011, 5(3):2316–2323. 10.1021/nn103596n
Liu Y, Das A, Xu S, Lin Z, Xu C, Wang ZL, Rohatgi A, Wong CP: Hybridizing zno nanowires with micropyramid silicon wafers as superhydrophobic high-efficiency solar cells. Adv Energy Mater 2012, 2(1):47–51. 10.1002/aenm.201100287
Zhang X, Pinion CW, Christesen JD, Flynn CJ, Celano TA, Cahoon JF: Horizontal silicon nanowires with radial p-n junctions: a platform for unconventional solar cells. J Phys Chem Lett 2013, 4(12):2002–2009. 10.1021/jz400533v
Kim S-K, Song K-D, Kempa TJ, Day RW, Lieber CM, Park H-G: Design of nanowire optical cavities as efficient photon absorbers. ACS Nano 2014, 4: 3707–3714.
Cao L, White JS, Park J-S, Schuller JA, Clemens BM, Brongersma ML: Engineering light absorption in semiconductor nanowire devices. Nat Mater 2009, 8(8):643–647. 10.1038/nmat2477
Hasan M, Huq MF, Mahmood ZH: A review on electronic and optical properties of silicon nanowire and its different growth techniques. SpringerPlus 2013, 2(1):151. 10.1186/2193-1801-2-151
Kayes BM, Atwater HA, Lewis NS: Comparison of the device physics principles of planar and radial p-n junction nanorod solar cells. J Appl Phys 2005, 97(11):114302. 10.1063/1.1901835
Kelzenberg MD, Putnam MC, Turner-Evans DB, Lewis NS, Atwater HA: Predicted efficiency of Si wire array solar cells. In Photovoltaic Specialists Conference (PVSC), 34th IEEE. Philadelphia, PA (USA): IEEE; 2009:001948–001953. ISBN: 978–1-4244–2949–3 ISBN: 978-1-4244-2949-3
Tian B, Kempa TJ, Lieber CM: Single nanowire photovoltaics. Chem Soc Rev 2009, 38(1):16–24. 10.1039/b718703n
Garnett E, Yang P: Light trapping in silicon nanowire solar cells. Nano Lett 2010, 10(3):1082–1087. 10.1021/nl100161z
Christesen JD, Zhang X, Pinion CW, Celano TA, Flynn CJ, Cahoon JF: Design principles for photovoltaic devices based on si nanowires with axial or radial p-n junctions. Nano Lett 2012, 12(11):6024–6029. 10.1021/nl303610m
Kempa TJ, Cahoon JF, Kim S-K, Day RW, Bell DC, Park H-G, Lieber CM: Coaxial multishell nanowires with high-quality electronic interfaces and tunable optical cavities for ultrathin photovoltaics. Proc Natl Acad Sci 2012, 109(5):1407–1412. 10.1073/pnas.1120415109
Wagner RS, Ellis WC: Vapor-liquid-solid mechanism of single crystal growth. Appl Phys Lett 1964, 4(5):89–90. 10.1063/1.1753975
Hung Y-J, Lee S-L, Thibeault BJ, Coldren LA: Realization of silicon nanopillar arrays with controllable sidewall profiles by holography lithography and a novel single-step deep reactive ion etching. In Materials Research Society Symposium Proceedings - MRS spring meeting. Warrendale, PA (USA): Materials Research Society; 2010. ISBN: 9781605112350 ISBN: 9781605112350
Hu L, Chen G: Analysis of optical absorption in silicon nanowire arrays for photovoltaic applications. Nano Lett 2007, 7(11):3249–3252. 10.1021/nl071018b
van de Groep J, Polman A: Designing dielectric resonators on substrates: combining magnetic and electric resonances. Opt Express 2013, 21(22):26285–26302. 10.1364/OE.21.026285
Zhu J, Yu Z, Burkhard GF, Hsu C-M, Connor ST, Xu Y, Wang Q, McGehee M, Fan S, Cui Y: Optical absorption enhancement in amorphous silicon nanowire and nanocone arrays. Nano Lett 2009, 9(1):279–282. 10.1021/nl802886y
Gueymard CA, Myers D, Emery K: Proposed reference irradiance spectra for solar energy systems testing. Solar Energy 2002, 73(6):443–467. 10.1016/S0038-092X(03)00005-7
Cheng Y-C, Chen T-G, Chang F-Y, Huang B-Y, Pan H-T, Li C-K, Yu P, Wu Y-R: Fabrication and modeling of large-scale silicon nanowire solar cells for thin-film photovoltaics. Photovoltaic Specialists Conference (PVSC), 38th IEEE 2012, 003083–003086. ISBN: 978–1-4673–0064–3 ISBN: 978-1-4673-0064-3
Fan Z, Kapadia R, Leu PW, Zhang X, Chueh Y-L, Takei K, Yu K, Jamshidi A, Rathore AA, Ruebusch DJ, Wu M, Javey A: Ordered arrays of dual-diameter nanopillars for maximized optical absorption. Nano Lett 2010, 10(10):3823–3827. 10.1021/nl1010788
Patchett S, Khorasaninejad M, O N, Saini SS: Effective index approximation for ordered silicon nanowire arrays. J Opt Soc Am B 2013, 30(2):306–313. 10.1364/JOSAB.30.000306
Li J, Yu H, Wong SM, Li X, Zhang G, Lo PG-Q, Kwong D-L: Design guidelines of periodic Si nanowire arrays for solar cell application. Appl Phys Lett 2009, 95(24):243113. 10.1063/1.3275798
Li J, Yu H, Li Y: Solar energy harnessing in hexagonally arranged Si nanowire arrays and effects of array symmetry on optical characteristics. Nanotechnology 2012, 23(19):194010. 10.1088/0957-4484/23/19/194010
Hong L, Wang X, Zheng H, Wang H, Yu H, Rusli: Design guidelines for slanting silicon nanowire arrays for solar cell application. J Appl Phys 2013, 114(8):084303. 10.1063/1.4819175
Lu Y, Lal A: High-efficiency ordered silicon nano-conical-frustum array solar cells by self-powered parallel electron lithography. Nano Lett 2010, 10(11):4651–4656. 10.1021/nl102867a
The authors declare that they have no competing interests.
SJ designed the studies, carried out the simulations, did the experiments, and drafted the manuscript. SS conceived the studies, advised on the entire project, and finalized the manuscript. Both authors read and approved the final manuscript.